Structural polymorphism and luminescence properties of zinc(ii) and cobalt(ii) MOFs with rigid and flexible ligands
Burlak, Pavel V.; Samsonenko, Denis G.; Kovalenko, Konstantin A.; Fedin, Vladimir P.; CrystEngComm 26 (2024) 5039–5045; doi:10.1039/D4CE00573B

data_7249229
_publ_section_title
;
 Structural polymorphism and luminescence properties of zinc(ii) and
 cobalt(ii) MOFs with rigid and flexible ligands
;
_journal_issue                   36
_journal_name_full               CrystEngComm
_journal_page_first              5039
_journal_page_last               5045
_journal_paper_doi               10.1039/D4CE00573B
_journal_volume                  26
_journal_year                    2024
_chemical_formula_sum            'C19 H19 Co N5 O6'
_chemical_formula_weight         472.32
_space_group_crystal_system      orthorhombic
_space_group_IT_number           73
_space_group_name_Hall           '-I 2b 2c'
_space_group_name_H-M_alt        'I b c a'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     dual
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-2019/3
_audit_update_record
;
2024-05-27 deposited with the CCDC.	2024-08-22 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   17.449(8)
_cell_length_b                   15.828(3)
_cell_length_c                   15.959(13)
_cell_measurement_reflns_used    3931
_cell_measurement_temperature    140(2)
_cell_measurement_theta_max      29.0
_cell_measurement_theta_min      3.0
_cell_volume                     4408(4)
_computing_cell_refinement       'XDS (Kabsch, 2010)'
_computing_data_collection       'Marccd (Doyle, 2011)'
_computing_data_reduction        'XDS (Kabsch, 2010)'
_computing_molecular_graphics    'ShelXle (H\"ubschle, 2011)'
_computing_publication_material  'CIFTAB (Sheldrick, 2015)'
_computing_structure_refinement  'SHELXL-2018 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT-2018 (Sheldrick, 2015)'
_diffrn_ambient_temperature      140(2)
_diffrn_detector_area_resol_mean 12.4
_diffrn_measured_fraction_theta_full 0.982
_diffrn_measured_fraction_theta_max 0.983
_diffrn_measurement_device_type  'Rayonix SX-165 CCD'
_diffrn_measurement_method       '\f scan'
_diffrn_radiation_monochromator  'Double Crystal Monochromator'
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     0.79313
_diffrn_reflns_av_R_equivalents  0.0953
_diffrn_reflns_av_unetI/netI     0.0529
_diffrn_reflns_Laue_measured_fraction_full 0.982
_diffrn_reflns_Laue_measured_fraction_max 0.983
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       19
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -19
_diffrn_reflns_number            13660
_diffrn_reflns_point_group_measured_fraction_full 0.982
_diffrn_reflns_point_group_measured_fraction_max 0.983
_diffrn_reflns_theta_full        28.417
_diffrn_reflns_theta_max         28.515
_diffrn_reflns_theta_min         3.299
_diffrn_source                   synchrotron
_exptl_absorpt_coefficient_mu    1.101
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.796
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'XDS (Kabsch, 2010)'
_exptl_crystal_colour            blue
_exptl_crystal_density_diffrn    1.424
_exptl_crystal_description       stick
_exptl_crystal_F_000             1944
_exptl_crystal_size_max          0.10
_exptl_crystal_size_mid          0.05
_exptl_crystal_size_min          0.05
_refine_diff_density_max         0.304
_refine_diff_density_min         -0.332
_refine_diff_density_rms         0.069
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.902
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     184
_refine_ls_number_reflns         1983
_refine_ls_number_restraints     72
_refine_ls_restrained_S_all      0.906
_refine_ls_R_factor_all          0.1374
_refine_ls_R_factor_gt           0.0779
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1929P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2281
_refine_ls_wR_factor_ref         0.2727
_reflns_Friedel_coverage         0.000
_reflns_number_gt                965
_reflns_number_total             1983
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d4ce00573b2.cif
_cod_data_source_block           bp389-3
_cod_depositor_comments
'Adding full bibliography for 7249228--7249230.cif.'
_cod_database_code               7249229
_shelx_shelxl_version_number     2019/3
_shelx_estimated_absorpt_t_min   0.898
_shelx_estimated_absorpt_t_max   0.947
_shelx_res_checksum              67204